its superplastic temperature of 970°C, re- sulting in a tight contact surface. The
higher welding temperature was also beneficial for atomic diffusion. Both ef-.
SUPPLEMENT TO THE WELDING JOURNAL, SEPTEMBER 1999 Sponsored by the American Welding Society and the Welding Research Council
Effects of Superplastic Deformation on the Diffusion Welding of SuperDux 65 Stainless Steel A two-stage diffusion process resulted in greatly improved weld strength BY M. S. YEH, Y. H. TSENG AND T. H. CHUANG
ABSTRACT. The SuperDux 651 stainless steel diffusion welded in a nonsuperplastic state (880°C, 60 min) required greater pressure, compared to aluminum and titanium alloys, to create a contact area at the weld interface, which will increase the atomic diffusion paths. However, an unsatisfactory weld strength of 45.3 MPa was obtained under the applied pressure of 7 MPa. This alloy deformed easily at its superplastic temperature of 970°C, resulting in a tight contact surface. The higher welding temperature was also beneficial for atomic diffusion. Both effects were advantageous for diffusion welding, while the joined workpieces macroscopically deformed markedly. In this study, a two-stage diffusion welding method was proposed. The specimens were diffusion welded in a nonsuperplastic (or superplastic) state for a short time and then further diffusion welded at superplastic (or nonsuperplastic) temperatures for a longer heating period. It was found that the welding strength could be improved drastically using such a twostage process. The contributions of superplastic deformation on the diffusion welding of this alloy during the two-stage process were clarified. M. S. YEH is with Department of Mechanical Engineering, Chung-Hua University, HsinChu, Taiwan, R.O.C. Y. H. TSENG and T. H. CHUANG are with Institute of Materials Science and Engineering, National Taiwan University, Taipei, Taiwan, R.O.C. 1. SuperDux 65 stainless steel is manufactured by Nippon Yakin Kogyo Co. Ltd, Japan.
Introduction Duplex stainless steels are Fe-Cr-Ni ternary alloys that possess a microstructure consisting of nearly equal amounts of ferrite and austenite. These stainless steels offer several advantages over the austenitic and ferritic stainless steels, namely, higher mechanical properties, good weldability, superior corrosion resistance and a lower price (Refs. 1–3). As a result, the duplex stainless steels have been widely used in the aerospace, chemical, power generation and oil and gas industries (Ref. 4). Good joining techniques are necessary for expanding the applications of duplex stainless steels. Fusion welding has been most commonly used. However, the heat-affected zone (HAZ) generated by fusion welding could reduce the mechanical properties and corrosion resistance of the joined workpieces (Refs. 1, 5). Diffusion welding is another choice. Because diffusion welding requires atomic diffusion at the weld interface for the transportation of el-
KEY WORDS Diffusion Welding SuperDux 65 Stainless Steel Superplastic Shear Strength
ements, material with a finer grain size provides a larger number of grain-boundary diffusion paths and, therefore, would possess better diffusion weldability. In addition, another necessary condition for satisfactory diffusion welding is intimate contact between the surfaces to be joined. Such intimate surface contact can be obtained in the conventional diffusion welding process by applying sufficient pressure, which causes microscopic plastic deformation at the contact surface between joined parts. It is well known that material with very fine grain size and a duplex structure will possess superplasticity at a certain strain rate (10-3~10-4 s-1) and higher temperature (>1⁄2Tm, where Tm is the melting point in degrees Kelvin). A superplastic material can be greatly deformed under very little applied stress. For this reason, intimate surface contact can be obtained easily during diffusion welding of a superplastic alloy. This implies a superplastic alloy can be diffusion welded under a lower applied normal pressure. Using the advantageous effect of superplasticity on diffusion welding, a twostage heating process was proposed. During such a process, the specimens were first diffusion welded at a nonsuperplastic (or superplastic) state for a short time and then further diffusion-welded at a superplastic (or nonsuperplastic) temperature for a longer heating period. The welding stage at superplastic temperatures (higher than 900°C) offered a beneficial effect of an intimate contact surface while the other stage at nonsuperplastic tempera-
WELDING RESEARCH SUPPLEMENT | 301-s
Fig. 1 — The dimensions of diffusion-welded specimens under applied pressure.
Fig. 3 — The welding interfaces of SuperDux 65 stainless steel subjected to various applied pressures at 880°C for 60 min. A — 7 MPa; B — 3.5 MPa; C — 2.1 MPa.
302-s | SEPTEMBER 1999
Fig. 2 — Microstructure of as-received SuperDux 65 stainless steel.
tures (lower than 900°C) was responsible mainly for atomic diffusion through the thermal effect. The lower temperatures in the nonsuperplastic heating stage offered the benefit of less energy consumption and material degradation. If manufactured properly, duplex stainless steels can Fig. 4 — Appearance of unwelded crevice at the specimen have a very fine edge after diffusion welding at 880°C for 60 min under 7 grain microstruc- MPa. ture, resulting in marked superplasticity (Ref. 6). Soylu, et al., detained at a pressure of 2.1 MPa after 4 h veloped two methods for reat 1007°C or 2 h at 1047°C. The purpose of this study was to evalfining the microstructure of uate the diffusion weldability of Super30Cr-8Ni steel. The first Dux 65 stainless steel using a monodimethod involved alloying durectional hot press method. Also, the plex stainless steels with copimprovement of diffusion welding per. The second method utithrough various two-stage processes was lized annealing of cold-rolled investigated. The information obtained supersaturated ferritic stainless in this study should also be useful for the steel (Ref. 7). On the other evaluation of the applicability of a conhand, Smith, et al., found that current superplastic forming/diffusion the superplastic elongation of welding (SPF/DW) technique for this cold-rolled IN744 steel alloy. This technique has been considreached 1050% at a strain rate ered as an advanced and economically of 3.2 x 10–4s-1 at 960°C (Ref. beneficial manufacturing process in the 8). The diffusion weldability of aerospace industry. However, most of the superplastic duplex stainless successful SPF/DW workpieces were tisteels had been evaluated by tanium alloys (Ref. 10). Information on Ridley and coworkers (Ref. 9) application of this technique to duplex using an isostatic pressure stainless steels was scarce. method with pressures of up to 2.8 MPa at a temperature beExperimental Procedure tween 927° and 1047°C for a long welding period (2–10 h). A SuperDux 65 stainless steel with a They found that a sound diffuthickness of 1 mm and the chemical sion-welded joint could be obcomposition as shown in Table 1 was
P AW where P is the breaking load, A is the overlap length and W is the sample width.
Results and Discussion The microstructure of as-received SuperDux 65 stainless steel in this study is shown in Fig. 2. This material possessed a rolling texture with a fine grain size of 6~7 µm. Figure 3 shows the interfacial microstructure of specimens after diffusion welding at 880°C for 60 min under various applied pressures from 2.1 to 7.0 MPa. The original contact surface representing the unwelded area was observed at all three applied pressures by optical microscopy, which revealed an unsatisfactory joint in this case. The shear strength (Table 2, A1–A3), which ranged only from 19.7 to 45.3 MPa, increased with increasing applied welding pressure. All of the specimens failed at the welding interface in
tensile shear tests. Figure 4 is the morphology of the specimen edge, which obviously shows an unwelded crevice. The superplastic deformation behavior of SuperDux 65 stainless steel appeared at about 900°C, which is above the welding temperature (880°C). In this stituation, diffusion welding for the SuperDux 65 stainless steel required greater normal pressure, which resulted in inti-
Fig. 5 — The welding interfaces of SuperDux 65 stainless steel conducted by using the two-stage welding method. A — 880°C/7 MPa/10 min + 970/7.0MPa/50 min; B — 970°C/3.5 MPa/10 min + 880°C/7 MPa/60 min; C — 970°C/3.5 MPa/10 min + 880°C/3.5 MPa/60 min.
WELDING RESEARCH SUPPLEMENT | 303-s
used in this study. Strips of this alloy with dimensions of 25 x 15 mm were cut from the as-received sheet material. The surfaces to be welded were prepared by grinding with 2000-grit SiC paper and polishing with 1-µm alumina powder, then cleaned by rinsing in distilled water, followed by ultrasonic cleaning in acetone for 5 min. Two strips of specimens were arranged with an overlap of 6T (T = 1-mm sheet thickness ), as shown in Fig. 1. Diffusion welding was carried out in a hot press under a vacuum of 4 x 10-4 Torr at various welding conditions. For A-type specimens, a single heating process at 880°C was used, which is below the superplastic deformation temperature of SuperDux 65 stainless steel (900°C). For comparison, various applied pressures (7.0, 3.5 and 2.1 MPa) were employed at the 880°C welding temperature. On the other hand, the B-type specimens were welded with a two-stage process: first, diffusion welded at a nonsuperplastic (or superplastic) state for 10 min, then further diffusion welded at a superplastic (or nonsuperplastic) temperature for a longer time. The welding conditions are shown in Table 2. After welding, the microstructure of the interface was observed using optical microscopy (OM) and scanning electron microscopy (SEM). In order to evaluate the welding efficiency, the average shear strength was determined from three welded specimens at room temperature with a crosshead speed of 1 mm/min. The shear strength (τ) was calculated by the equation
diffusion-welding step (970°C, 3.5MPa) for only 10 min, when added to the singlestage process at a nonsuperplastic state, obviously improved the welding effect of this alloy, while resulting in a welding strength of approximately 76 MPa. In this case, sufficiently initimate surface contact had formed at the initial stage of diffusion Fig. 6 — The microstructure at the specimen edge for SuperDux 65 stainless steel joined by the two-stage welding process. welding in a superA — 880°C/7 MPa/10 min + 970°C/7 MPa/50 min; B — 970°C/3.5 MPa/10 min + 880°C/3.5M Pa/60 min. plastic state such that the further increase of the applied stress B2 and B3 specimens were lower than mate contact, promoting atomic diffufrom 3.5 to 7.0 MPa at the second stage that of the B1 specimen, they were apsion paths for a sound joint. For the dif(880°C, 60 min) did not markedly inproximately twice as high as those of the fusion welding in a nonsuperplastic crease the welding strength. A1 and A2 specimens. From Table 2, it state, increasing the applied load will can be seen that B2 and B3 specimens cause more contact area to be plastically References were joined with an additional stage in deformed, which results in higher weldthe superplastic range (970°C/3.5 ing strength. 1. Nilsson, J.-O. 1992. Super duplex stainMPa/10 min) during their diffusion weldThe SuperDux 65 stainless steels less steels. Materials Science and Technology 8(8): 685–700. ing processes in comparison with speciwere further diffusion welded with a 2. Potgieter, J. H., Premachandra, K., Jackmens A1 and A2. The effect of greater two-stage process. The microstructures son, E. M. L. E. M., and Nana, S. 1991.Duplex: surface contact through superplastic deof the welding interface are shown in Complex or Simplex. FWP J. 31(1): 17–29. formation at the initial stage (even for a Fig. 5. Experimental results showed the 3. Fibf, R. C., and Nicholls, J. M. 1993. short time) on the strength of diffusiontwo-stage welding process had a better High performance super duplex stainless steel welded SuperDux 65 stainless steel was effect than the conventional single-stage castings. The Foundryman (7): 228–232. thus demonstrated. That the weld diffusion welding method (Table 2). The 4. Davison, R. M., and Redmond, J. D. 1991. A guide to using duplex stainless steels. strengths of B2 and B3 specimens were most obvious improvement was obMaterials & Design 12(4): 187–192. similar implied that the initial diffusion tained in B1 specimens, which were 5. Atamert, S., and King, J. E. 1992. Super welding at a superplastic state (970 welded in the following condition: 880 duplex stainless steels — part 1: heat affected °C/3.5 MPa/10 min) had resulted in °C/7.0 MPa/ 10 min + 970°C/7.0 zone microstructures. Materials Science and greater surface contact than when the MPa/50 min. Original contact surface Technology 8(10): 896–911. first welding stage was nonsuperplastic. was still visible in the joined specimens 6. Maehara, Y., and Langdon, T. G. 1990. Thus, a higher applied load for the B2 as shown in Fig. 5A and the shear weldSuperplasticity of steels and ferrous alloys. Materials Science and Engineering A128: specimen in comparison with the B1 ing strength increased to 132.2 MPa. In 1–13. specimen at the second stage played a comparison with the excellent joint in 7. Soylu, B., and Honeycombe, R. W. K. minor role in the welding effect. the B1 specimen, the B2 and B3 speci1991. Microstructural refinement of duplex mens revealed a discontinuous weld instainless steels. Materials Science and Techterface (Fig. 5B and C), which possessed Conclusions nology 7(2): 137–145. shear welding strengths of 75.0 and 76.7 8. Smith, C. I., Norgate, B., and Ridley, N. 1976. Mat. Sci. 10: 182. MPa, respectively. The microstructures An obvious residue of the original 9. Ridley, N., Salehi, M. T., and Pilling, J. of the specimen edge for SuperDux 65 weld interface and lack of welding at the 1992. Isostatic diffusion bonding of microdustainless steel joined by the two-stage specimen edge was observed for the conplex stainless steel. Materials Science and process are shown in Fig. 6. The unventional single-stage diffusion welding Technology 8(9): 791–795. welded edge crevices appearing in the of SuperDux 65 stainless steel at 880°C for 10. Hamilton, C. H., and Ascani, L. A. specimens diffusion welded with a sin60 min under applied pressures from 2.1 1975. Method for superplastic forming of metgle-stage process in a nonsuperplastic to 7.0 MPa. The weld strengths were very als with concurrent diffusion bonding. United States Patent No. 3-920-175. state were absent when at least part of low, ranging from 19.7 to 45.3 MPa. On the welding was performed near superthe other hand, in the SuperDux 65 stainplastic conditions. This proves that the less steel welded using a two-stage diffuapplied pressure during the superplastic sion welding process, the original interdiffusion-welding stage effectively inface largely disappeared and the weld creased the contact area and accelerated strength increased drastically. Diffusion atomic diffusion. Furthermore, a near welding under the condition of 880°C/7.0 macroscopic deformation was observed MPa/10 min + 970°C/7.0 MPa/50 min rein the welding condition used for specisulted in a dramatically higher welding men B1: 880°C/7.0 MPa/ 10 min + 970 strength of 132.2 MPa, in which macro°C/7.0MPa /50 min. scopic deformation of such a specimen Although the welding strengths of the was noted. Using an initial superplastic
304-s | SEPTEMBER 1999